Once you have dried your design thoroughly your PMC/ Art Clay Silver design will be ready to fire.
The advantage of the PMC3, PMC+ and Art Clay is that you can fire it with either a kiln, a gas torch or even on your hob! On this page we go into detail about each process so that you can decide which one will work best for you and your design.
To get used to the firing process we recommend that you first try a little experiment. Take a small pea sized piece of PMC and roll it out into a rod. On one end of the rod concentrate the heat in an effort to melt it. This will allow you recognise the signs so you don't damage an important piece later on.
Ensure your clay is completely dry before firing; if it isn’t you might find it may break or explode during firing, resulting in injury or burns. Use a hair dryer, dehydrator, warming plate, or kitchen oven to dry the clay. To check if the piece is completely dry, place the warm piece on cold stainless steel or a cold mirror. After about 10 to 20 seconds remove the piece. If there is no water condensation on the plate you are using, the piece is probably dry - please note this test isn’t 100% reliable but should give you some indication.
To help see if your piece has fired successfully, trace the outline of the unfired piece on a sheet of paper. Compare the fired piece with the traced size - Art Clay Silver contracts 8-10% in volume after firing so you should see a slight shrinkage.
Prepare a bowl of water to cool off the piece after firing. The bowl should be made of stainless steel or glass.
Tim McCreight, author & experienced metalsmith recommends the following method for firing with a gas torch, we have used this method successfully & found it easy to follow.
1. Place your work on a soldering block on a fireproof surface.
2. Light the torch & hold the flame about 2cm away from your work (depending on the size of your piece and heat of the flame).
3. Within a minute the piece will be enveloped in a soft flame as the binder burns away. The flame will soon go out by itself. Within another minute, the piece will start to glow red (You will only be able to see the change of colour in dim light).
4. Continue heating until this becomes a bright & luminous colour. At this point glance at a clock.
5. Hold this colour as uniformly as possible. For PMC+ hold for at least 5 minutes. For PMC3, hold the temperature for about 2 minutes.
6. When the time is up, turn off the torch & allow to cool.
For this method you will need a Gas Hob Firing Mesh With Cover. The mesh sheet measures approximately 16 x 16cm - large enough for most projects. It comes with a smaller piece of mesh, ready shaped for you to make a cage to cover your piece during firing for extra safety - (fold this into a box shape by bending the edges over prior to starting the firing process).
Read the following method thoroughly before starting to ensure a correct and safe firing.
1. Place the stainless steel mesh on over the gas hob. Make sure it is stable and secure. Turn on the hob and find the hottest area by checking where the glow is the strongest. It is easier to see this if you dim the lights. Turn the hob off.
2. Immediately place your design on the hottest part of the firing mesh using a pair of tweezers. Place the protective cover over the metal clay.
3. Turn the hob back on. Your metal clay will flame for a few seconds as the binder in the clay burns off. Soon the piece will begin to glow. Fire for 5 minutes. For safety, don’t move or touch your piece or the mesh.
4. After firing for 5 minutes, turn off the hob and let the piece cool on the mesh for about 15 minutes. If you try to remove the piece before it is cool it may stick to the mesh. When the piece is cool it will easily detach from the mesh.
5. Once your design has cooled on the mesh, pick it up with tweezers and dip into water to ensure it is completely cool. Then dry the piece.
6. Check the size of the fired piece against the outline of the unfired piece. If it hasn't contracted, the piece has not been successfully fired. Repeat steps 5 – 8.
The Paragon SC2 kiln is one of the most popular and recommended kilns for using with all types of metal clay. It gives you lot's of control in terms of setting temperatures - allowing you to take more time over heating your metal clay, which helps to make it stronger in the long run.
The digital programmer allows you to easily control the temperature, ramping (the rate at which the kiln heats up) and the time the temperature is held. It heats up in approximately 15-20 minutes. The elements are embedded in ceramic fibre and heat the kiln from both sides, minimising the front-to-back temperature difference common with smaller kilns.
The amount of time you decide to heat your design for will depend on how strong you need the piece to be. A good general rule for firing pieces comprising only of metal clay is 900°C (any higher than this and the metal clay begins to distort) for two hours. This will make your design really strong. If you are including any gemstones in the piece, a different program is needed. The shortest time and heat that can be used for PMC3 is 10 minutes at 650, but firing at a higher temperature for longer will improve the strength.
Have you made any jewellery using metal clay? We would love to see your creations. Find us on Facebook, Twitter, Instagram and Google +. Just search Kernowcraft.
For any further advice regarding the contents on this page or for any other general jewellery making enquires, please feel free to get in touch, we would love to hear from you.
If you have any further questions, feel free to call our friendly team who will be more than happy to give you some advice through Facebook, Twitter, Email or simply calling us on 01872 573888 8.30am-4.30pm.
Alternatively, for more information and how to's on all areas of jewellery making visit our other Gemstone Setting Advice pages.